# this file is part of refractiveindex.info database
# refractiveindex.info database is in the public domain
# copyright and related rights waived via CC0 1.0

REFERENCES: "<a href=\"http://refractiveindex.info/download/data/2017/ohara_2017-11-30.agf\">OHARA Zemax catalog 2017-11-30</a> (obtained from <a href=\"http://www.ohara-inc.co.jp/en/product/optical/list/\">http://www.ohara-inc.co.jp</a>)<br>See also <a href=\"http://refractiveindex.info/download/data/2017/ohara_2017-11-30.pdf\">OHARA glass data sheets</a>"
COMMENTS: "Recommended - Lightweight "
DATA:
  - type: formula 2 
    range: 0.37 2.4
    coefficients: 0 1.55849775 0.0115367235 0.230767007 0.0586095947 1.84436099 162.981888
  - type: tabulated k
    data: |
        0.370 5.7890E-06
        0.380 2.2195E-06
        0.390 1.0195E-06
        0.400 5.5498E-07
        0.420 2.1036E-07
        0.440 1.2838E-07
        0.460 9.6434E-08
        0.480 7.3273E-08
        0.500 5.6098E-08
        0.550 2.6340E-08
        0.600 2.8734E-08
        0.650 3.6335E-08
        0.700 2.7922E-08
        0.800 1.2745E-08
        0.900 7.1656E-09
        1.000 7.9617E-09
        1.200 9.5541E-09
        1.400 5.5844E-08
        1.600 6.3822E-08
        1.800 1.7293E-07
        2.000 3.2154E-07
        2.200 1.0460E-06
        2.400 1.3655E-06
SPECS:
    n_is_absolute: false
    λ_is_vacuum: false
    temperature: 25.0 °C
    coefficients_of_thermal_dispersion: 4.7e-07 1.25e-08 -3.4e-11 8.29e-07 1.09e-09 0.289
    n_d: 1.698947
    V_d: 30.127865
    glass_code: 699301
    density: 2.96 g/cm<sup>3</sup>
    coefficient_of_thermal_expansion_1: 7.5e-06 K<sup>-1</sup>
    coefficient_of_thermal_expansion_2: 8.9e-06 K<sup>-1</sup>
    ΔP_gF: 0.0103
    climatic_resistance: 1.0
    acid_resistance: 1.0
    phosphate_resistance: 1.0
